#------------------------------------------------------------------------------
#$Date: 2016-03-24 02:29:14 +0200 (Thu, 24 Mar 2016) $
#$Revision: 179581 $
#$URL: svn://www.crystallography.net/cod/cif/4/50/46/4504670.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4504670
loop_
_publ_author_name
'Wang, Jing-Ping'
'Zhao, Jun-Wei'
'Duan, Xian-Ying'
'Niu, Jing-Yang'
_publ_section_title
;
 Syntheses and Structures of One- and Two-Dimensional
 Organic−Inorganic Hybrid Rare Earth Derivatives Based on
 Monovacant Keggin-Type Polyoxotungstates
;
_journal_issue                   2
_journal_name_full               'Crystal Growth & Design'
_journal_page_first              507
_journal_paper_doi               10.1021/cg050433j
_journal_volume                  6
_journal_year                    2006
_chemical_formula_sum            'C6 H53 N2 O99 Si2 Sm5 W22'
_chemical_formula_weight         6590.13
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                108.09(3)
_cell_angle_beta                 90.69(3)
_cell_angle_gamma                107.79(3)
_cell_formula_units_Z            1
_cell_length_a                   12.894(3)
_cell_length_b                   13.193(3)
_cell_length_c                   20.591(4)
_cell_measurement_reflns_used    250
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      25
_cell_measurement_theta_min      2.5
_cell_volume                     3148.2(15)
_computing_cell_refinement       Raxis
_computing_data_collection       Raxis
_computing_data_reduction        Raxis
_computing_molecular_graphics    Texsan
_computing_publication_material  Texsan
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.714
_diffrn_measured_fraction_theta_max 0.714
_diffrn_measurement_device_type  R-axis-IV
_diffrn_measurement_method       'Osillation frames'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0000
_diffrn_reflns_av_sigmaI/netI    0.1449
_diffrn_reflns_limit_h_max       14
_diffrn_reflns_limit_h_min       -15
_diffrn_reflns_limit_k_max       15
_diffrn_reflns_limit_k_min       0
_diffrn_reflns_limit_l_max       22
_diffrn_reflns_limit_l_min       -22
_diffrn_reflns_number            7927
_diffrn_reflns_theta_full        25.00
_diffrn_reflns_theta_max         25.00
_diffrn_reflns_theta_min         1.72
_diffrn_standards_decay_%        none
_diffrn_standards_interval_count none
_diffrn_standards_interval_time  none
_diffrn_standards_number         none
_exptl_absorpt_coefficient_mu    22.400
_exptl_absorpt_correction_T_max  0.2674
_exptl_absorpt_correction_T_min  0.0679
_exptl_absorpt_correction_type   empirical
_exptl_crystal_colour            Colorless
_exptl_crystal_density_diffrn    3.476
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       Block
_exptl_crystal_F_000             2861
_exptl_crystal_size_max          0.26
_exptl_crystal_size_mid          0.12
_exptl_crystal_size_min          0.08
_refine_diff_density_max         3.317
_refine_diff_density_min         -2.820
_refine_diff_density_rms         0.499
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.023
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     676
_refine_ls_number_reflns         7927
_refine_ls_number_restraints     412
_refine_ls_restrained_S_all      0.999
_refine_ls_R_factor_all          0.1031
_refine_ls_R_factor_gt           0.0798
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0836P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1640
_refine_ls_wR_factor_ref         0.1782
_reflns_number_gt                6093
_reflns_number_total             7927
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            cg050433jsi20050822_015609.cif
_cod_data_source_block           njy1
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Triclinic' changed to 'triclinic'
according to /home/saulius/struct/CIF-dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.1 from
2010-06-29.

'_exptl_absorpt_correction_type' value 'Empirical'
changed to 'empirical' according to
/home/saulius/struct/CIF-dictionaries/cif_core.dic dictionary named
'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_values 1715 2011-07-08 13:25:40Z adriana 
;
_cod_original_cell_volume        3148.1(11)
_cod_original_sg_symbol_H-M      P-1
_cod_database_code               4504670
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Sm1 Sm -0.06935(11) 0.15707(11) 0.63612(6) 0.0254(3) Uani 1 1 d .
Sm2 Sm -0.40121(12) -0.13718(12) 0.84943(7) 0.0333(4) Uani 1 1 d .
Sm3 Sm 0.0085(2) 0.5486(2) 0.98569(11) 0.0201(6) Uani 0.50 1 d PU
Si1 Si 0.1603(6) 0.0657(7) 0.7493(3) 0.0272(16) Uani 1 1 d U
W1 W 0.26022(11) -0.15935(10) 0.65284(5) 0.0401(3) Uani 1 1 d .
W2 W -0.00144(11) -0.22108(9) 0.68724(5) 0.0404(4) Uani 1 1 d .
W3 W 0.07487(10) -0.08424(9) 0.57335(5) 0.0298(3) Uani 1 1 d .
W4 W 0.34492(9) -0.00751(9) 0.84015(5) 0.0289(3) Uani 1 1 d .
W5 W 0.07992(9) -0.06707(9) 0.87290(5) 0.0291(3) Uani 1 1 d .
W6 W 0.24678(9) 0.20106(9) 0.92425(4) 0.0260(3) Uani 1 1 d .
W7 W 0.44360(10) 0.13965(10) 0.71402(5) 0.0309(3) Uani 1 1 d .
W8 W 0.25663(9) 0.20786(9) 0.63017(5) 0.0272(3) Uani 1 1 d .
W9 W 0.34430(8) 0.34447(8) 0.79832(5) 0.0229(3) Uani 1 1 d .
W10 W -0.11518(9) 0.01085(9) 0.77172(5) 0.0293(3) Uani 1 1 d .
W11 W 0.04696(8) 0.27520(8) 0.82686(4) 0.0210(3) Uani 1 1 d .
O1 O 0.3312(18) -0.245(2) 0.6224(11) 0.057(6) Uani 1 1 d U
O2 O -0.1008(19) -0.354(2) 0.6743(11) 0.061(6) Uani 1 1 d U
O3 O 0.0415(13) -0.1335(16) 0.4849(8) 0.030(4) Uani 1 1 d U
O4 O 0.4523(17) -0.053(2) 0.8614(10) 0.050(5) Uani 1 1 d U
O5 O 0.0113(17) -0.149(2) 0.9181(11) 0.051(5) Uani 1 1 d U
O6 O 0.2873(14) 0.2850(17) 1.0070(8) 0.031(4) Uani 1 1 d U
O7 O 0.5774(16) 0.145(2) 0.7064(10) 0.046(5) Uani 1 1 d U
O8 O 0.2880(15) 0.2563(18) 0.5609(9) 0.037(4) Uani 1 1 d U
O9 O 0.4077(13) 0.4830(15) 0.8403(8) 0.026(4) Uani 1 1 d U
O10 O -0.2331(13) -0.0530(16) 0.7989(8) 0.027(4) Uani 1 1 d U
O11 O 0.0303(13) 0.3945(15) 0.8904(8) 0.026(4) Uani 1 1 d U
O12 O 0.1929(16) -0.156(2) 0.5731(10) 0.046(5) Uani 1 1 d U
O13 O -0.0763(12) 0.1593(15) 0.8383(7) 0.022(3) Uani 1 1 d U
O14 O 0.3275(14) 0.3499(17) 0.7085(8) 0.032(4) Uani 1 1 d U
O15 O -0.1588(13) 0.0521(16) 0.7066(8) 0.027(4) Uani 1 1 d U
O16 O 0.0480(15) -0.1671(18) 0.7868(9) 0.038(4) Uani 1 1 d U
O17 O 0.4672(14) 0.2895(16) 0.7733(8) 0.030(4) Uani 1 1 d U
O18 O 0.3759(16) -0.0184(19) 0.6650(10) 0.044(5) Uani 1 1 d U
O19 O -0.0202(17) -0.221(2) 0.5966(10) 0.053(5) Uani 1 1 d U
O20 O -0.0860(13) -0.1190(16) 0.7165(8) 0.028(4) Uani 1 1 d U
O21 O 0.4045(14) 0.1877(17) 0.6441(8) 0.034(4) Uani 1 1 d U
O22 O -0.0083(14) -0.0085(17) 0.6007(9) 0.034(4) Uani 1 1 d U
O23 O -0.0268(15) -0.0163(18) 0.8517(9) 0.038(4) Uani 1 1 d U
O24 O 0.1227(14) 0.2333(17) 0.8959(9) 0.036(4) Uani 1 1 d U
O25 O 0.1992(15) 0.0528(18) 0.5878(9) 0.038(4) Uani 1 1 d U
O26 O 0.3346(12) 0.2864(15) 0.8757(7) 0.021(3) Uani 1 1 d U
O27 O -0.0137(13) 0.2763(15) 0.7533(8) 0.025(4) Uani 1 1 d U
O28 O 0.1216(13) 0.2207(15) 0.6434(8) 0.024(4) Uani 1 1 d U
O29 O 0.2950(15) -0.1159(18) 0.7511(9) 0.039(5) Uani 1 1 d U
O30 O 0.3578(14) 0.1273(17) 0.9191(8) 0.032(4) Uani 1 1 d U
O31 O 0.2282(12) -0.0839(15) 0.8760(8) 0.023(4) Uani 1 1 d U
O32 O 0.1500(12) 0.0734(14) 0.9490(7) 0.020(3) Uani 1 1 d U
O33 O 0.4160(13) 0.0913(16) 0.7950(8) 0.025(4) Uani 1 1 d U
O34 O 0.1954(11) 0.3314(14) 0.8084(7) 0.016(3) Uani 1 1 d U
O35 O 0.123(2) -0.261(3) 0.6638(14) 0.084(8) Uani 1 1 d U
O36 O 0.1991(12) 0.0486(15) 0.8211(7) 0.023(4) Uani 1 1 d U
O37 O 0.0543(13) 0.1042(15) 0.7593(8) 0.024(4) Uani 1 1 d U
O38 O 0.2666(12) 0.1595(14) 0.7311(7) 0.017(3) Uani 1 1 d U
O39 O 0.1387(14) -0.0545(17) 0.6886(9) 0.035(4) Uani 1 1 d U
O1W O -0.2349(18) 0.217(2) 0.6482(11) 0.053(5) Uani 1 1 d U
O2W O -0.2348(17) 0.002(2) 0.5658(10) 0.050(5) Uani 1 1 d U
O3W O -0.0314(19) 0.342(2) 0.6146(11) 0.059(6) Uani 1 1 d U
O4W O -0.324(2) 0.072(3) 0.9179(13) 0.078(8) Uani 1 1 d U
O5W O -0.2270(13) -0.1027(16) 0.9192(8) 0.028(4) Uani 1 1 d U
O6W O -0.347(3) -0.272(3) 0.7520(16) 0.092(8) Uani 1 1 d U
O7W O -0.4495(17) -0.103(2) 0.7465(10) 0.053(6) Uani 1 1 d U
O8W O -0.4198(16) -0.315(2) 0.8757(10) 0.047(5) Uani 1 1 d U
O9W O -0.457(3) -0.108(3) 0.9649(17) 0.035(8) Uani 0.50 1 d PU
O10W O 0.000(5) 0.612(6) 0.882(3) 0.096(16) Uani 0.50 1 d PU
O11W O 0.080(2) 0.775(3) 1.0260(14) 0.0206(13) Uani 0.50 1 d PU
N1 N -0.734(3) -0.408(4) 0.7344(19) 0.049(7) Uani 0.50 1 d PDU
N2 N 0.358(4) 0.605(4) 1.019(2) 0.057(6) Uani 0.50 1 d PDU
O1A O -0.575(2) -0.285(3) 0.8043(13) 0.018(6) Uani 0.50 1 d PDU
O2A O 0.211(3) 0.613(3) 0.9737(18) 0.041(9) Uani 0.50 1 d PDU
C1 C -0.620(4) -0.327(5) 0.7438(17) 0.052(14) Uani 0.50 1 d PDU
H1A H -0.5858 -0.3102 0.7073 0.063 Uiso 0.50 1 calc PR
C2 C -0.741(5) -0.521(4) 0.738(3) 0.049(7) Uani 0.50 1 d PDU
H2A H -0.8170 -0.5664 0.7335 0.074 Uiso 0.50 1 calc PR
H2B H -0.7058 -0.5122 0.7819 0.074 Uiso 0.50 1 calc PR
H2C H -0.7059 -0.5578 0.7019 0.074 Uiso 0.50 1 calc PR
C3 C -0.784(5) -0.363(4) 0.798(2) 0.049(7) Uani 0.50 1 d PDU
H3A H -0.7826 -0.2876 0.8028 0.073 Uiso 0.50 1 calc PR
H3B H -0.7422 -0.3614 0.8374 0.073 Uiso 0.50 1 calc PR
H3C H -0.8582 -0.4102 0.7945 0.073 Uiso 0.50 1 calc PR
C4 C 0.267(4) 0.548(4) 0.961(3) 0.057(6) Uani 0.50 1 d PDU
H4A H 0.2544 0.4804 0.9253 0.068 Uiso 0.50 1 calc PR
C5 C 0.396(6) 0.718(4) 1.074(3) 0.057(6) Uani 0.50 1 d PDU
H5A H 0.3345 0.7450 1.0840 0.086 Uiso 0.50 1 calc PR
H5B H 0.4500 0.7701 1.0575 0.086 Uiso 0.50 1 calc PR
H5C H 0.4269 0.7123 1.1143 0.086 Uiso 0.50 1 calc PR
C6 C 0.436(4) 0.542(6) 0.993(3) 0.057(6) Uani 0.50 1 d PDU
H6A H 0.3971 0.4700 0.9596 0.085 Uiso 0.50 1 calc PR
H6B H 0.4713 0.5316 1.0305 0.085 Uiso 0.50 1 calc PR
H6C H 0.4909 0.5847 0.9715 0.085 Uiso 0.50 1 calc PR
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Sm Sm -0.1638 3.4418 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O28 Sm1 O15 120.3(6) . .
O28 Sm1 O27 76.5(5) . .
O15 Sm1 O27 72.6(6) . .
O28 Sm1 O22 72.2(6) . .
O15 Sm1 O22 77.4(6) . .
O27 Sm1 O22 115.9(6) . .
O28 Sm1 O3 78.6(5) . 2_556
O15 Sm1 O3 140.7(6) . 2_556
O27 Sm1 O3 146.2(6) . 2_556
O22 Sm1 O3 76.9(6) . 2_556
O28 Sm1 O1W 144.4(7) . .
O15 Sm1 O1W 81.3(7) . .
O27 Sm1 O1W 85.0(7) . .
O22 Sm1 O1W 143.3(7) . .
O3 Sm1 O1W 102.8(6) 2_556 .
O28 Sm1 O2W 141.8(7) . .
O15 Sm1 O2W 71.5(6) . .
O27 Sm1 O2W 138.1(6) . .
O22 Sm1 O2W 76.1(7) . .
O3 Sm1 O2W 73.8(6) 2_556 .
O1W Sm1 O2W 68.9(8) . .
O28 Sm1 O3W 77.8(7) . .
O15 Sm1 O3W 143.6(7) . .
O27 Sm1 O3W 83.1(7) . .
O22 Sm1 O3W 138.5(7) . .
O3 Sm1 O3W 69.5(7) 2_556 .
O1W Sm1 O3W 69.8(8) . .
O2W Sm1 O3W 115.3(7) . .
O7W Sm2 O1A 78.0(8) . .
O7W Sm2 O9W 137.3(11) . .
O1A Sm2 O9W 89.1(11) . .
O7W Sm2 O4 67.4(7) . 1_455
O1A Sm2 O4 70.8(10) . 1_455
O9W Sm2 O4 69.9(10) . 1_455
O7W Sm2 O5W 135.6(6) . .
O1A Sm2 O5W 139.0(9) . .
O9W Sm2 O5W 78.2(9) . .
O4 Sm2 O5W 136.1(7) 1_455 .
O7W Sm2 O6W 73.6(10) . .
O1A Sm2 O6W 78.7(10) . .
O9W Sm2 O6W 143.7(12) . .
O4 Sm2 O6W 134.3(9) 1_455 .
O5W Sm2 O6W 88.9(8) . .
O7W Sm2 O8W 132.5(8) . .
O1A Sm2 O8W 65.5(9) . .
O9W Sm2 O8W 73.4(11) . .
O4 Sm2 O8W 122.3(7) 1_455 .
O5W Sm2 O8W 73.5(6) . .
O6W Sm2 O8W 70.4(9) . .
O7W Sm2 O10 68.8(6) . .
O1A Sm2 O10 135.3(7) . .
O9W Sm2 O10 135.6(9) . .
O4 Sm2 O10 118.9(7) 1_455 .
O5W Sm2 O10 66.9(5) . .
O6W Sm2 O10 64.1(9) . .
O8W Sm2 O10 118.5(7) . .
O7W Sm2 O4W 93.1(8) . .
O1A Sm2 O4W 140.4(10) . .
O9W Sm2 O4W 71.5(11) . .
O4 Sm2 O4W 70.1(8) 1_455 .
O5W Sm2 O4W 71.6(8) . .
O6W Sm2 O4W 136.1(10) . .
O8W Sm2 O4W 134.4(8) . .
O10 Sm2 O4W 72.1(7) . .
Sm3 Sm3 O11 75.3(4) 2_567 .
Sm3 Sm3 O10W 148.4(17) 2_567 .
O11 Sm3 O10W 76.1(17) . .
Sm3 Sm3 O11 68.9(4) 2_567 2_567
O11 Sm3 O11 144.2(3) . 2_567
O10W Sm3 O11 138.4(17) . 2_567
Sm3 Sm3 O2A 105.0(9) 2_567 .
O11 Sm3 O2A 76.3(10) . .
O10W Sm3 O2A 80.8(16) . .
O11 Sm3 O2A 112.7(9) 2_567 .
Sm3 Sm3 O11W 141.1(6) 2_567 .
O11 Sm3 O11W 136.6(7) . .
O10W Sm3 O11W 70.5(18) . .
O11 Sm3 O11W 76.7(7) 2_567 .
O2A Sm3 O11W 71.9(12) . .
O37 Si1 O39 113.2(10) . .
O37 Si1 O36 109.1(9) . .
O39 Si1 O36 106.3(10) . .
O37 Si1 O38 113.1(10) . .
O39 Si1 O38 106.8(9) . .
O36 Si1 O38 108.0(8) . .
O1 W1 O12 103.0(10) . .
O1 W1 O29 102.9(10) . .
O12 W1 O29 154.1(9) . .
O1 W1 O35 102.3(13) . .
O12 W1 O35 89.2(10) . .
O29 W1 O35 86.4(10) . .
O1 W1 O18 97.9(11) . .
O12 W1 O18 92.6(9) . .
O29 W1 O18 82.7(8) . .
O35 W1 O18 158.7(12) . .
O1 W1 O39 173.0(9) . .
O12 W1 O39 73.2(8) . .
O29 W1 O39 81.2(8) . .
O35 W1 O39 72.0(11) . .
O18 W1 O39 88.3(8) . .
O2 W2 O35 101.5(13) . .
O2 W2 O19 96.3(10) . .
O35 W2 O19 86.6(11) . .
O2 W2 O20 102.4(10) . .
O35 W2 O20 156.1(11) . .
O19 W2 O20 90.2(9) . .
O2 W2 O16 103.0(9) . .
O35 W2 O16 92.9(10) . .
O19 W2 O16 160.4(9) . .
O20 W2 O16 82.4(8) . .
O2 W2 O39 171.7(9) . .
O35 W2 O39 73.1(11) . .
O19 W2 O39 77.3(8) . .
O20 W2 O39 83.0(7) . .
O16 W2 O39 83.8(7) . .
O22 W3 O3 102.7(9) . .
O22 W3 O25 91.0(9) . .
O3 W3 O25 102.5(8) . .
O22 W3 O12 161.4(8) . .
O3 W3 O12 95.8(8) . .
O25 W3 O12 83.6(9) . .
O22 W3 O19 94.4(9) . .
O3 W3 O19 99.7(8) . .
O25 W3 O19 155.3(8) . .
O12 W3 O19 83.7(9) . .
O22 W3 O39 90.8(8) . .
O3 W3 O39 165.7(8) . .
O25 W3 O39 81.7(7) . .
O12 W3 O39 70.8(7) . .
O19 W3 O39 74.2(7) . .
O4 W4 O31 103.0(9) . .
O4 W4 O33 101.3(9) . .
O31 W4 O33 155.6(7) . .
O4 W4 O29 97.9(10) . .
O31 W4 O29 91.2(7) . .
O33 W4 O29 86.0(8) . .
O4 W4 O30 103.6(9) . .
O31 W4 O30 87.5(7) . .
O33 W4 O30 86.3(7) . .
O29 W4 O30 158.2(8) . .
O4 W4 O36 174.9(7) . .
O31 W4 O36 72.4(7) . .
O33 W4 O36 83.2(7) . .
O29 W4 O36 84.7(7) . .
O30 W4 O36 74.1(7) . .
O5 W5 O16 101.0(10) . .
O5 W5 O23 99.6(10) . .
O16 W5 O23 87.5(9) . .
O5 W5 O32 99.4(9) . .
O16 W5 O32 159.4(7) . .
O23 W5 O32 92.2(8) . .
O5 W5 O31 102.9(9) . .
O16 W5 O31 88.7(8) . .
O23 W5 O31 157.4(7) . .
O32 W5 O31 83.7(7) . .
O5 W5 O36 171.0(8) . .
O16 W5 O36 83.4(7) . .
O23 W5 O36 88.4(7) . .
O32 W5 O36 76.0(6) . .
O31 W5 O36 69.0(6) . .
O6 W6 O26 102.7(8) . .
O6 W6 O24 105.8(9) . .
O26 W6 O24 90.3(7) . .
O6 W6 O30 95.5(8) . .
O26 W6 O30 86.4(7) . .
O24 W6 O30 158.7(8) . .
O6 W6 O32 93.8(7) . .
O26 W6 O32 162.5(7) . .
O24 W6 O32 90.8(7) . .
O30 W6 O32 86.2(7) . .
O6 W6 O36 164.6(8) . .
O26 W6 O36 87.2(6) . .
O24 W6 O36 85.7(7) . .
O30 W6 O36 73.1(7) . .
O32 W6 O36 75.4(6) . .
O7 W7 O21 104.9(8) . .
O7 W7 O17 99.2(9) . .
O21 W7 O17 86.0(8) . .
O7 W7 O18 97.8(10) . .
O21 W7 O18 95.4(8) . .
O17 W7 O18 161.9(8) . .
O7 W7 O33 101.8(8) . .
O21 W7 O33 153.2(7) . .
O17 W7 O33 87.6(7) . .
O18 W7 O33 83.1(8) . .
O7 W7 O38 172.0(9) . .
O21 W7 O38 73.0(6) . .
O17 W7 O38 73.1(6) . .
O18 W7 O38 90.1(7) . .
O33 W7 O38 80.2(6) . .
O8 W8 O28 102.3(8) . .
O8 W8 O25 102.7(9) . .
O28 W8 O25 92.4(8) . .
O8 W8 O14 100.3(8) . .
O28 W8 O14 91.5(8) . .
O25 W8 O14 155.3(7) . .
O8 W8 O21 94.7(8) . .
O28 W8 O21 162.5(6) . .
O25 W8 O21 87.8(8) . .
O14 W8 O21 81.3(8) . .
O8 W8 O38 164.4(7) . .
O28 W8 O38 91.7(6) . .
O25 W8 O38 83.5(7) . .
O14 W8 O38 72.0(6) . .
O21 W8 O38 70.9(6) . .
O9 W9 O14 98.8(8) . .
O9 W9 O34 101.6(8) . .
O14 W9 O34 91.5(7) . .
O9 W9 O17 102.4(8) . .
O14 W9 O17 88.4(7) . .
O34 W9 O17 155.7(8) . .
O9 W9 O26 100.1(7) . .
O14 W9 O26 161.0(8) . .
O34 W9 O26 83.5(6) . .
O17 W9 O26 88.7(7) . .
O9 W9 O38 173.8(6) . .
O14 W9 O38 75.7(7) . .
O34 W9 O38 81.7(6) . .
O17 W9 O38 74.8(7) . .
O26 W9 O38 85.4(6) . .
O10 W10 O15 104.0(8) . .
O10 W10 O20 98.7(8) . .
O15 W10 O20 98.8(8) . .
O10 W10 O13 100.0(8) . .
O15 W10 O13 93.4(8) . .
O20 W10 O13 154.4(7) . .
O10 W10 O23 87.9(7) . .
O15 W10 O23 167.8(7) . .
O20 W10 O23 82.1(8) . .
O13 W10 O23 81.4(7) . .
O10 W10 O37 167.7(6) . .
O15 W10 O37 86.7(7) . .
O20 W10 O37 85.4(7) . .
O13 W10 O37 72.8(6) . .
O23 W10 O37 81.2(6) . .
O27 W11 O11 102.8(8) . .
O27 W11 O13 94.2(7) . .
O11 W11 O13 99.5(7) . .
O27 W11 O34 96.3(6) . .
O11 W11 O34 102.8(7) . .
O13 W11 O34 152.4(7) . .
O27 W11 O24 163.8(9) . .
O11 W11 O24 93.3(8) . .
O13 W11 O24 81.7(7) . .
O34 W11 O24 81.1(6) . .
O27 W11 O37 84.2(8) . .
O11 W11 O37 169.1(6) . .
O13 W11 O37 71.4(6) . .
O34 W11 O37 84.5(6) . .
O24 W11 O37 79.7(7) . .
W3 O3 Sm1 157.5(9) . 2_556
W4 O4 Sm2 161.0(11) . 1_655
W10 O10 Sm2 175.2(9) . .
W11 O11 Sm3 174.3(9) . .
W11 O11 Sm3 138.6(9) . 2_567
Sm3 O11 Sm3 35.8(3) . 2_567
W1 O12 W3 123.5(11) . .
W11 O13 W10 118.4(8) . .
W9 O14 W8 119.9(10) . .
W10 O15 Sm1 134.9(8) . .
W5 O16 W2 155.3(13) . .
W7 O17 W9 120.9(9) . .
W7 O18 W1 150.0(11) . .
W2 O19 W3 117.8(11) . .
W10 O20 W2 156.0(9) . .
W7 O21 W8 123.5(8) . .
W3 O22 Sm1 158.4(10) . .
W5 O23 W10 146.4(10) . .
W6 O24 W11 148.6(9) . .
W8 O25 W3 146.9(11) . .
W6 O26 W9 147.9(9) . .
W11 O27 Sm1 138.6(10) . .
W8 O28 Sm1 156.0(10) . .
W4 O29 W1 152.8(12) . .
W6 O30 W4 119.3(8) . .
W4 O31 W5 124.3(9) . .
W5 O32 W6 116.5(7) . .
W4 O33 W7 153.8(9) . .
W9 O34 W11 160.6(10) . .
W2 O35 W1 124.6(18) . .
Si1 O36 W4 126.6(9) . .
Si1 O36 W5 122.5(8) . .
W4 O36 W5 94.2(6) . .
Si1 O36 W6 119.8(10) . .
W4 O36 W6 93.5(5) . .
W5 O36 W6 91.5(5) . .
Si1 O37 W10 130.4(10) . .
Si1 O37 W11 126.8(9) . .
W10 O37 W11 94.0(6) . .
Si1 O38 W9 125.0(8) . .
Si1 O38 W8 121.6(8) . .
W9 O38 W8 92.3(6) . .
Si1 O38 W7 125.0(9) . .
W9 O38 W7 91.2(5) . .
W8 O38 W7 92.3(5) . .
Si1 O39 W1 129.2(10) . .
Si1 O39 W2 122.4(9) . .
W1 O39 W2 90.1(7) . .
Si1 O39 W3 122.0(11) . .
W1 O39 W3 92.3(6) . .
W2 O39 W3 90.3(6) . .
C1 N1 C3 106(4) . .
C1 N1 C2 115(5) . .
C3 N1 C2 100.4(9) . .
C4 N2 C5 134(5) . .
C4 N2 C6 100.6(9) . .
C5 N2 C6 121(5) . .
C1 O1A Sm2 128(3) . .
C4 O2A Sm3 123(4) . .
O1A C1 N1 115(4) . .
O1A C1 H1A 122.6 . .
N1 C1 H1A 122.6 . .
N1 C2 H2A 109.5 . .
N1 C2 H2B 109.5 . .
H2A C2 H2B 109.5 . .
N1 C2 H2C 109.5 . .
H2A C2 H2C 109.5 . .
H2B C2 H2C 109.5 . .
N1 C3 H3A 109.5 . .
N1 C3 H3B 109.5 . .
H3A C3 H3B 109.5 . .
N1 C3 H3C 109.5 . .
H3A C3 H3C 109.5 . .
H3B C3 H3C 109.5 . .
O2A C4 N2 102(4) . .
O2A C4 H4A 128.8 . .
N2 C4 H4A 128.8 . .
N2 C5 H5A 109.5 . .
N2 C5 H5B 109.5 . .
H5A C5 H5B 109.5 . .
N2 C5 H5C 109.5 . .
H5A C5 H5C 109.5 . .
H5B C5 H5C 109.5 . .
N2 C6 H6A 109.5 . .
N2 C6 H6B 109.5 . .
H6A C6 H6B 109.5 . .
N2 C6 H6C 109.5 . .
H6A C6 H6C 109.5 . .
H6B C6 H6C 109.5 . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Sm1 O28 2.333(16) .
Sm1 O15 2.381(15) .
Sm1 O27 2.392(16) .
Sm1 O22 2.45(2) .
Sm1 O3 2.459(16) 2_556
Sm1 O1W 2.48(2) .
Sm1 O2W 2.50(2) .
Sm1 O3W 2.52(3) .
Sm2 O7W 2.41(2) .
Sm2 O1A 2.42(3) .
Sm2 O9W 2.44(3) .
Sm2 O4 2.45(2) 1_455
Sm2 O5W 2.492(16) .
Sm2 O6W 2.50(3) .
Sm2 O8W 2.51(2) .
Sm2 O10 2.513(15) .
Sm2 O4W 2.54(3) .
Sm3 Sm3 1.530(5) 2_567
Sm3 O11 2.439(18) .
Sm3 O10W 2.53(6) .
Sm3 O11 2.530(15) 2_567
Sm3 O2A 2.53(4) .
Sm3 O11W 2.69(3) .
Si1 O37 1.592(19) .
Si1 O39 1.63(2) .
Si1 O36 1.655(16) .
Si1 O38 1.678(15) .
W1 O1 1.64(3) .
W1 O12 1.869(19) .
W1 O29 1.930(17) .
W1 O35 1.93(3) .
W1 O18 1.94(2) .
W1 O39 2.37(2) .
W2 O2 1.77(3) .
W2 O35 1.86(3) .
W2 O19 1.88(2) .
W2 O20 1.943(19) .
W2 O16 1.975(18) .
W2 O39 2.373(19) .
W3 O22 1.67(2) .
W3 O3 1.732(16) .
W3 O25 1.953(19) .
W3 O12 2.02(2) .
W3 O19 2.05(2) .
W3 O39 2.375(17) .
W4 O4 1.77(2) .
W4 O31 1.841(15) .
W4 O33 1.856(16) .
W4 O29 1.898(19) .
W4 O30 1.96(2) .
W4 O36 2.291(17) .
W5 O5 1.70(2) .
W5 O16 1.803(19) .
W5 O23 1.81(2) .
W5 O32 1.961(16) .
W5 O31 1.993(16) .
W5 O36 2.334(15) .
W6 O6 1.689(17) .
W6 O26 1.870(14) .
W6 O24 1.905(19) .
W6 O30 1.95(2) .
W6 O32 1.979(15) .
W6 O36 2.344(17) .
W7 O7 1.71(2) .
W7 O21 1.864(17) .
W7 O17 1.90(2) .
W7 O18 1.92(2) .
W7 O33 1.963(15) .
W7 O38 2.394(15) .
W8 O8 1.740(17) .
W8 O28 1.815(17) .
W8 O25 1.86(2) .
W8 O14 1.997(19) .
W8 O21 2.033(19) .
W8 O38 2.368(13) .
W9 O9 1.687(18) .
W9 O14 1.886(16) .
W9 O34 1.894(14) .
W9 O17 1.947(19) .
W9 O26 1.961(14) .
W9 O38 2.291(16) .
W10 O10 1.693(15) .
W10 O15 1.741(16) .
W10 O20 1.887(19) .
W10 O13 1.919(18) .
W10 O23 2.171(18) .
W10 O37 2.219(15) .
W11 O27 1.703(15) .
W11 O11 1.780(18) .
W11 O13 1.915(15) .
W11 O34 1.919(14) .
W11 O24 2.016(18) .
W11 O37 2.285(19) .
O3 Sm1 2.459(16) 2_556
O4 Sm2 2.45(2) 1_655
O11 Sm3 2.530(15) 2_567
N1 C1 1.497(10) .
N1 C3 1.498(10) .
N1 C2 1.499(10) .
N2 C4 1.491(10) .
N2 C5 1.496(10) .
N2 C6 1.500(10) .
O1A C1 1.247(10) .
O2A C4 1.254(10) .
C1 H1A 0.9300 .
C2 H2A 0.9600 .
C2 H2B 0.9600 .
C2 H2C 0.9600 .
C3 H3A 0.9600 .
C3 H3B 0.9600 .
C3 H3C 0.9600 .
C4 H4A 0.9300 .
C5 H5A 0.9600 .
C5 H5B 0.9600 .
C5 H5C 0.9600 .
C6 H6A 0.9600 .
C6 H6B 0.9600 .
C6 H6C 0.9600 .
